CATALYSIS TODAY CatalysisToday 27 (1996) 41--47
NO reduction by C H 4 o v e r rare earth oxides Xiankuan Zhang, Arden B. Waiters, M. Albert Vannice * Department of Chemical Engineering, The Pennsylvania State University, University Park, PA 16802, USA
Abstract NO reduction by methane was studied between 773 and 973 K. All the REO catalysts tested were active for this reaction in both the absence and presence of 02. Activities increased continuously with reaction temperature and no deactivation or bend-over was observed at high temperatures except for Sm203, over which complete combustion of CH4 occurred in the presence of 02. The specific activities for NO reduction to N2 by CH4 were higher than those for NO decomposition, showing that CH4 enhances NO conversion. CHa reduction of NO gave selectivities to N2 that were near 100% for all the catalysts except Sr/La203, Sm203 and Sr/Sm203, over which 5-20% N20 was formed. Except for CeO2, the presence of 02 promoted the rate of NO conversion to N2. Overall, Sr/La203 had the highest specific activity for NO reduction by CH4 in either the absence or presence of O2, with respective values 0f4.6 X 10 -3 and 13 × 10-3/×mole N2/s/m 2 at 773 K. Turnover frequencies (TOFs) under these two sets of conditions, based on NO adsorption at 300 K, were 0.78 × 10 -3 s- l and 2.3 X 10 -3 s- i, respectively. Activation energies fell between 22-32 kcal/mole for all the REOs. The best REO catalysts correlated with those best for the oxidative coupling of methane. On either a specific activity or a TOF basis, the best REO catalysts were comparable to Co-ZSM-5. Keywords: Nitrogenoxide; Methane;Rare earth oxides
Metal ion-exchanged ZSM-5 catalysts have been shown to be active for selective reduction of NO by CH4 and the presence of excess oxygen actually enhanced activities for NO reduction [ 1]. However, the zeolite-based catalysts showed a volcano-like activity dependency on temperature and at higher temperatures NO reduction was severely decreased, which could limit the suitability of these zeolite catalysts for some applications. We have successfully prepared and characterized two non-zeolitic catalyst systems (Li/MgO and L a 2 0 3 ) for NO reduction by CH4 [2,3]. Li/MgO and La203 were chosen because * Correspondingauthor. 0920-5861/96/$32.00 © 1996 ElsevierScienceB.V. All rights reserved SSD10920-5861 (95) 00170-0
they were two of the best catalyst systems for the methane oxidative coupling (MOC). The results showed both Li/MgO and La203 w e r e active for NO reduction by CH4. Unlike the zeolites, the activities of these catalysts continuously increased with reaction temperature. In this paper we present the results of NO reduction by CH4 in both absence and presence of O2 over a series of rare earth oxide (REO) catalysts. In order to make comparisons, the corresponding results obtained over Li/MgO and Co-ZSM-5 are also included and discussed. 2. Experimental
The pure rare earth oxide samples, La203, CeO2, Nd203, Sm203, Tm203, Lu203, were pre-
X. Zhang et al. /Catalysis Today 27 (1996) 41--47
pared by calcining the corresponding commercial oxides at 1023 K for 10 h under flowing dry air ( ~ 50 sccm) . The doped samples of 4 wt.-% Sr/La203 and 4 wt.-% Sr/Sm203 were prepared by following the preparation of the Li/MgO samples . All the activity measurements and kinetic studies were made at atmospheric pressure under steady-state reaction conditions in a quartz microreactor. The microreactor system has been described in detail in a previous paper . A typical gas mixture, unless otherwise specified, of 2% NO and 0.5% CH4 in He at a stoichiometric ratio of NO:CH4 = 4:1, according to the reaction: 4NO + CH 4 ~ 2N2 + C O 2 + 2H20, was passed through the reactor which contained ca. 100 mg catalyst. All the gases used were from MG Ind., UHP Grade, except for the NO mixed with He, which was 99.0 ÷ % with major mixture impurities of N2 (ca. 600 ppm), N20 (ca. 100 ppm) and CO2 (ca. 100 ppm). The reactor effluent was analyzed with a gas chromatograph (Perkin-Elmer Sigma-2B) equipped with a Carboxen t°°° column (Supelco) and a P-E Nelson 1020S integrator . During the Arrhenius runs, a period of 30 rain on stream was allowed at each temperature before any gas sample was taken. An ascendingdescending temperature sequence from 773 to 973 K was typically used to check for any deactivation during these measurements. Runs with no catalyst verified that no reaction occurred over this temperature range. The conversions were generally
kept below 20% to ensure differential reactor operation.
The reaction of NO reduction by CH4 over these rare earth oxides was studied between 773 and 973 K using a stoichiometric NO/CH4 ratio of 2.0% NO, 0.51% CH4 in He at a total flow rate of 40 ml/(STP)/min (20 ml/min for La203). All the REO catalysts were active for NO reduction by CH4 at 773 K, the activities continuously increased with temperature, and no deactivation was observed over a period of 30 h. The corresponding activation energies are presented in Table 1. N and C mass balances were within + 2.5% thus indicating that little or no NO2 was formed although the GC column used did not separate NO2 as a well-defined peak . Except for a small amount of N20 in the product stream whose concentration was routinely near that of the impurity N20 level in the feed (ca. 100 ppm), dinitrogen was essentially the only N-containing product detected over La203 , LU203, CeO2, Nd203, and Tm203. Therefore, the net rate of N20 formation was near zero and the selectivities of NO conversion to N2 were close to 100%. However, noticeable amounts of NEt were observed over Sr/La203, Sm203 and Sr/Sm203, particularly at low temperature and selectivity to N 2 dropped to 80-95% at lower temperatures but increased with temperature.
Table 1 NO Reduction by CH4 at 773 K (No 02), Pr = 1 atm, PNo = 15.4 Torr and
Rate o f N 2 Formation (/xmol/s/g × 10~)
Specific Activity (/~mol/s/m2 × 103)
TOF (s-J × 103)
La203 Sr/La203 CeO 2 Nd203 Sm203 Sr/Sm203 Tm203 Lu2Oa Li/MgO Co-ZSM-5
24 26 28 22 32 28 28 22 31 -
5.3 7.8 1.3 4.9 15 11 1.0 6.8 1.8 332
1.5 4.6 0.54 1.4 2. l 1.6 1.1 2.8 0.50 1.7
0.39 0.78 0.31 0.54 0.46 0.51 0.19 0.56 0.67 0.59
X. Zhan g et al. / Catalysis Today 27 (1996) 41-47 15
o~ ~ •.~
6 8 8 ~
8 8 8
Catalyst Fig. 1. Specific activities: ( shaded square) NO decomposition (from Ref. ), (IS]) NO reduction by CH4 and (11) NO reduction by CH4 in the presence of 02; (a) T= 773 K and (b) T= 973 K, partial pressure as stated in results section.
Table 1 also summarizes the rates, specific activities and turnover frequencies (TOFs) at 773 K for N2 formation during NO reduction by CH4 in the absence of 02 over the REOs as well as Li/ MgO and Co-ZSM-5. The TOFs (molecules N2/ s/site) are based on the number of NO molecules irreversibly adsorbed at 300 K . The specific activities obtained at both 773 K and 973 K are presented in Fig. 1. On a gram basis, Sr/La203, Sm203 and Sr/Sm203 were the most active cata-
lysts at both 773 and 973 K, although they were much less active than Co-ZSM-5 at 773 K. When specific activities and TOFs are compared, Sr/ La203 was clearly the most active and was even more active than Co-ZSM-5. Li/MgO had a low specific activity, but the TOFs on all these surfaces, including Li/MgO and Co-ZSM-5, are remarkably similar, with the possible exception of Tm203. Every rate of N2 formation via CH 4 reduction was higher than the corresponding rate for direct NO decomposition [ 4 ], as shown in Fig. 1a, indicating CH 4 enhances the activity for NO conversion to N2. The effect of dioxygen on the activity and selectivity of NO reduction by CH 4 on the REOs was also investigated between 773 and 973 K using a mixture of 1.8% NO (2.0% for La203), 0.45% CH 4 (0.51% for La203) and 1.0% 02 in He at a total flow rate of 44.5 ml (STP) / min ( 40 ml / min for La203). Again it was found that all the REOs were active at 773 K, the rates of N2 formation continuously increased with temperature up to 973 K, and no bend-over behavior was observed except for Sm203 after all the CH 4 had combusted. The corresponding activation energies, presented in Table 2, varied from 22 to 29 kcal/mol and were quite similar to those in the absence of 02. Because of NO2 formation downstream from the reactor due to the gas-phase reaction between NO and 02, the selectivity of NO conversion to N2 could not be quantitatively determined in these experiments. The effect of dioxygen on the activity and selectivity of NO reduction by CH 4 on the REOs was examined and Table 2 also summarizes the rates, specific activities, and TOFs at 773 K for N2 formation via NO reduction by CH4 in the presence of 02, while specific activities obtained at 773 K and 973 K are presented in Fig. 1. On a gram basis, La203 was the most active catalyst while CeO2, much less active than all the other REOs, and CoZSM-5 was again 1-2 orders of magnitude more active. However, the specific activities of all the REOs except CeO2 were comparable to that of Co-ZSM-5, with Sr/La203 having the highest value, which was double that of Co-ZSM-5. A
X. Zhang et al. / Catalysis Today 27 (1996) 41-47
Table 2 NO Reduction by CH4 at 773 K in the presence of 1% O2, Pr = 1 atm, PNo = 13.8 Torr and Pc,4 = 3.5 Torr Catalyst
Rate o f N 2 Formation (/~mol/s/g × 1 0 3 )
Specific Activity (~mol/s/m2 × 103)
TOF ( s - t × 103)
La203 Sr/La203 CeO2 Nd203 Sm~O3 Sr/Sm203 Tm203 Lu203 Li/MgO Co-ZSM-5
26 26 28 22 23 29 25 22 35 -
30 22 0.75 23 25 21 2.7 18 0.84 1280
8.5 13 0.30 6.7 3.5 3.2 2.9 7.3 0.24 6.6
2.2 2.3 0.17 2.5 0.77 1.0 0.49 1.4 0.32 2.3
comparison of TOFs shows almost identical values on La203, Sr/La203, Nd203 and Co-ZSM-5 at 773 K. Specific activities and TOFs in this reaction were higher in the presence of 02 than in its absence, thus indicating that 02 facilitates NO reduction to N2 except for the two worst catalysts (CeO2 and Li/MgO) whose activities were somewhat lower in the presence of 02. In the presence of 02, methane can react not only with nitric oxide but also with O2 via combustion as follows: 4NO +
C H 4 --~ 2N2 +
CO2 + 2H20
Total methane conversion frequently increased rapidly with temperature and the selectivity of CH4 reacting with NO, i.e., the fraction of CH4 100
Z O 3o
'0 C m
850 900 Temperature (K)
CH4 + 202 ~ CO2 + 2H20
reaction with NO vs. the total c n 4 reacted, typically decreased as temperature increased before reaching a nearly constant value. Fig. 2 shows an example of total NO and CH4 conversion, and the selectivity of CH4 reacting with NO vs. 02. No higher hydrocarbons due to the oxidative coupling of methane were detected in the presence of 02 under any circumstances.
0 1000 ,
Fig. 2. NO conversion (O), CI-I4 conversion ( 0 ) , selectivity for CH4 reacting with NO (El) and with 02 ( 1 ) over Sr/La203.
This study has confirmed that certain REOs and promoted REOs are quite active for NO× reduction. For comparison, the activity of each REO for NO conversion to Na in this study is expressed in three different ways: (1) a rate, /xmol N2/s/g; (2) a specific activity,/zmol N2/s/m2; and (3) a turnover frequency (TOF), molecule N2/site/s. T m 2 0 3 had a very low BET surface area and C e O 2 had a very low irreversible NO uptake which could have led to a high specific activity and a high TOF, respectively, although their rates are among the lowest. At these high temperatures, activities over Co-ZSM-5 become much less favorable in comparison with REOs because they severely decrease with increasing temperature above 700-800 K [ 1,4]. At lower temperatures the zeolite catalysts are more active. A comparison of the rates for NO reduction by CH4 (see Table 1 and Table 2) and those for direct NO decomposition  shows that CH4 clearly enhances the NO conversion, as illustrated
X. Zhang et al. / Catalysis Today 27 (1996) 41-47
in Fig. la, for example, the activity over Sr/La203 increased by a factor of 5.5 while the respective activation energies for these two reactions remained quite similar. CeO2, Sm203 and Lu203 showed a somewhat larger variation in Ea values. The promotional effect of CH4 on NO conversion to N2 might be expected on the basis that CH4 can facilitate the removal of surface oxygen left behind by the decomposition of nitrogen oxide species. This would be particularly apparent if the rate-determining step were the removal of surface oxygen. Indeed, CO2 was observed instead of 02 in the presence of CH4, indicating an interaction between CH4 and surface oxygen. CO was not detected in these experiments, partly because its peak overlaps with NO in the chromatogram so that even if some CO were formed it would be obscured by the large NO peak. On the other hand, CO, once formed, could rapidly react with NO to produce N2 and CO2. The selectivity of NO conversion to N2, rather than N20, was essentially 100% over La203, Lu203, CeO2, Nd203 and Tm203. However Sr/La203, Sm203 and Sr/ Sm203 produced noticeable amounts of N20 under the same conditions, i.e., 5 to 20% of the product was N20. The N mass balance indicated that there were only small amounts, if any, of other N-containing compounds such as NO2. As proposed previously, N20 could be an intermediate during NO reduction by methane ; thus the amount of N20 in the products would depend on the relative rates of NO conversion and N20 decomposition to N2. Interestingly, N20 was observed only with the most active catalysts for NO reduction. Over these catalysts the rate of N20 decomposition may not be significantly higher than that of NO reduction thus resulting in some undecomposed N20, while over other catalysts the rate of N20 decomposition was presumably much higher than the rate of NO reduction, which resulted in no N20 detected in the reaction products [ 3 ]. Perhaps of greater importance, the presence of excess O2 promotes NO reduction by CH4 over all the catalysts except CeO2 and Li/MgO (see Table 1 and Table 2), and the magnitude of the
activity increase differs. For example, the activity on La203 at 773 K increased by a factor of about 6 in the presence of dioxygen, while that of Sm203 increased less than 2-fold. As discussed in a previous paper [ 2 ], the role of dioxygen in NO reduction by CH 4 over the rare earth oxides is not likely due to the formation of NO2 as an intermediate, as suggested for zeolite catalysts [5,6], rather it is presumed to promote the activation of methane via the formation of methyl radicals, which are presumed to remain on the surface at these lower temperatures. Chajar et al. recently reported that as reduction of NO2 by propane occurred over a Cu/MFI zeolite catalyst, a partial decomposition of NO2 created 02 which was responsible for an increase in activity via the partial oxidation of propane . It is not known why the presence of excess dioxygen inhibits NO conversion to N2 over CeO2 and Li/MgO under the same conditions; however, CeO2 is not a good methane oxidative coupling catalyst. Total CH 4 conversion on CeO2 varied from ca. 1% at 773 K to ca. 35% at 973 K, which was much lower than CH 4 conversions over other REOs. Therefore, the activity decrease in the presence of 02 is not due to a much lower CH 4 concentration caused by combustion. It is perhaps surprising that CeO2 has the lowest activity for both direct NO decomposition and reduction by CH4 in the absence of oxygen as CeO2 has been widely used as a promoter in threeway automotive exhaust catalysts [ 8 ]. Correlations between catalytic activity and properties of the rare earth oxides have always been interesting subjects because of gradual changes caused by the lanthanide contraction. Takasu et al. found similarities between activity for NO oxidation to NO2 and that for isotopic oxygen exchange suggesting that the rate-determining process of each reaction was closely related [ 9 ]. In a study of CO hydrogenation over REO-supported Pd, Vannice et al. found the CH 4 turnover frequency decreased as the activation energy for electrical conductivity increased in the REO support, whereas the CH3OH turnover frequency was dependent on the atomic number of the REOs and decreased with the lanthanide con-
X. Zhang et al. / Catalysis Today 27 (1996) 41-47
traction [ 10]. In the present work no correlation could be found between any catalytic activity and a given property of the REOs, such as electron configuration, covalent and ionic radii, or activation energy for electron conductivity. However, we have found that, in general, good methane oxidative coupling catalysts are also good NO reduction catalysts. For example, La203 and Sm203 are two of the best catalyst systems reported for methane oxidative coupling [ 11,12]. Doping La203 with strontium improves both activity and selectivity for oxidative coupling [ 12], and our study has shown it also provides a significant increase in specific activity for NO reduction by CH4. Nd203 is a moderately active catalyst for this reaction [ 13 ], while CeO2 is completely non-selective for C2 hydrocarbon formation, although it is active for total oxidation to CO2 [ 12]. The conversion to N2 over Li/MgO is lowered because of the high selectivity to N20 . All these observations are consistent with the present results for NO reduction by CH4 over these REOs and support our belief that these two reactions are closely related in terms of methane activation, presumably involving methyl radicals . It is well known that methyl radicals can be generated on the surface of Li/MgO catalysts during methane oxidative coupling . Control experiments performed over both Li/MgO and La203 [2,3] verified that the catalysts prepared in this study are indeed methane oxidative coupling catalysts, which implies that they can generate methyl radicals under appropriate conditions. However, no C2 hydrocarbons were detected over the REOs under any circumstances during NO reduction by CH4 in the presence of 02. The absence of any detectable amount of C2 hydrocarbons may imply one of several possibilities: ( 1) once generated, all methyl radicals on the surface react rapidly with NO before they can desorb into the gas phase and couple to form C2H6, (2) methyl radicals do desorb but react rapidly with NO in the gas phase and (3) any C2 hydrocarbons formed by coupling of methyl radicals react further with NO, as it has been reported that higher hydrocarbons are more reactive with NO than CH4
during NO reduction over zeolite catalysts [ 15 ]. The first explanation is preferred. It is important to compare these REO catalysts with other catalysts which can also reduce NO to N2 by CH4. A number of zeolite catalysts have been studied, and Co-ZSM-5, Ga-H-ZSM-5 and Ga/H-mordenite have been found to be the most active for NO reduction by CH4 in the presence of 02 [ 1,16,17]. When the reaction was conducted at 773 K in a gas mixture of 1610 ppm NO, 1000 ppm CH4 and 2.5% 02 at a GHSV of 30 000 h - 1, the rates of N2 formation over Co-ZSM-5 and GaZSM-5 were 0.18 and 0.20 /.tmol/s/g, respectively, which are about 1-2 orders of magnitude higher than those of the REO catalysts at the same temperature after correction for the NO pressure dependence [ 1]. The rate of N2 formation over Co-ZSM-5 is enhanced at higher NO concentrations . When compared in terms of either specific activity or TOF, the REOs are comparable to Co-ZSM-5 for NO reduction by CH4 in the presence of 02, as shown in Table 2 and Fig. 1. Furthermore, the activity of each REO continuously increased with reaction temperature, except for Sm203, and the activities at 973 K are about 20-30 times higher than those at 773 K, whereas both Co-ZSM-5 and Ga/H-ZSM-5 showed a decrease in activity above 773 K, particularly for Co-ZSM-5 [ 1]. It was suggested that the decrease in NO conversion did not happen until almost all the CH 4 was combusted, thus this behavior can be attributed to CH4 depletion [ 17] ; our results support this explanation . Nevertheless, dioxygen promotes NO reduction to N2 by CH 4 on both the zeolite and REO catalysts (except for CeO2) which may indicate similar chemistry associated with the formation of reaction intermediates involving oxygen.
5. Summary This study has shown that NO reduction by CH4 can occur readily on both pure REOs and Sr-promoted REO surfaces. Furthermore, the rate of NO reduction by CH4 was enhanced 2- to 6-fold by
X. Zhang et al. / Catalysis Today 27 (1996) 41-47
the presence of 02 over all the REOs examined except CeO2. In the absence of 02, the relative specific activities for NO reduction by CH 4 are: Sr/La203 > Lu203 > Sm203 > Sr/Sm203, La203, Nd203 > Tm203 > CeO2. However, the TOF values are all rather similar, except possibly for Tm203. In the presence of 1% 02, a much wider variation (over 40-fold) in specific activity occurred for NO reduction by CH 4 and the relative order at 773 K was Sr/La203 > La203 > Lu203 > Nd203 > Sm203 > Sr/Sm203 > Tm203 > CeO2. The addition of 02 had little effect on the apparent activation energy except for Sm203. These results have been discussed in greater detail elsewhere . The surface chemistry associated with these catalytic processes is not yet understood and studies are underway in our laboratory to gain additional insight; however, the positive influence of both promoters and 02 coupled with the capability to determine both specific activities and TOFs provides optimism that further improvements are possible.
Acknowledgements This work was supported by the National Science Foundation under Grant No. CTS-9211552.
We would like to thank Dr. Y. Li and Dr. J. Armor for providing samples of metal-ZSM-5 catalysts.
References [ 1 ] Y. Li and J.N. Armor, J. Catal., 145 (1994) 1.  X. Zhang, A.B. Waiters and M.A. Vannice, J. Catal., 146 (1994) 568.  X. Zhang, A.B. Walters and M.A. Vannice, Appl. Catal. B, 4 (1994) 237.  X. Zhang, A.B. Waiters and M.A. Vannice, J. Catal., 155 (1995) 290.  G.P. Ansell, A.F. Diwell, S.E. Golunski, J.W. Hayes, R.R. Rajaram, T.J. Truex and A.P. Walker, Appl. Catal. B, 2 (1993) 81.  J. Valyon and W.K. Hall, J. Phys. Chem., 97 (1993) I204.  Z. Chajar, M. Primet, H. Praliaud, M. Chevrier, C. Gauthier and F. Mathis, Catal. Lett., 28 (1994) 33.  B. Harris, A.F. Diwell and C. Hallet, Platinum Met. Rev., 32 (1988) 73.  T. Takasu, S. Nishibe and Y. Matsuda, J. Catal., 49 (1977) 236.  M.A. Vannice, C. Sudhakar and M. Freeman, J. Catal., 108 (1987) 97. [ 11 ] J.M. Deboy and R.F. Hicks, J. Catal., 113 (1988) 517. [ 12] S. Sugiyama, Y. Matsumura and J.B. Moffat, J. Catal., 139 (1993) 338.  K. Otsuka, K. Jinno and A. Morikawa, Chem. Lett., (1985) 499. [ 14] T. Ito and J.H. Lunsford, Nature, 314 (1985) 721. [ 15] M. Iwamoto and H. Hamada, Catal. Today, 10 ( 1991 ) 57. [ 16] K. Yogo, M. Ihara, I. Terasaki and E. Kikuchi, Chem. Lett., (1993) 229. [ 17] Y. Li and J.N. Armor, Appl. Catal., B2 (1993) 239.